Photoresponse of indium oxide particulate-based thin films ... sawyes/ The photoresponse
Embed Size (px)
Transcript of Photoresponse of indium oxide particulate-based thin films ... sawyes/ The photoresponse
Photoresponse of indium oxide particulate-based thin films fabricated using milled nanorods
grown by the self-catalytic vapor–liquid–solid process
This article has been downloaded from IOPscience. Please scroll down to see the full text article.
2012 Semicond. Sci. Technol. 27 045005
IP Address: 184.108.40.206
The article was downloaded on 20/04/2012 at 21:59
Please note that terms and conditions apply.
View the table of contents for this issue, or go to the journal homepage for more
Home Search Collections Journals About Contact us My IOPscience
http://iopscience.iop.org/page/terms http://iopscience.iop.org/0268-1242/27/4 http://iopscience.iop.org/0268-1242 http://iopscience.iop.org/ http://iopscience.iop.org/search http://iopscience.iop.org/collections http://iopscience.iop.org/journals http://iopscience.iop.org/page/aboutioppublishing http://iopscience.iop.org/contact http://iopscience.iop.org/myiopscience
IOP PUBLISHING SEMICONDUCTOR SCIENCE AND TECHNOLOGY
Semicond. Sci. Technol. 27 (2012) 045005 (6pp) doi:10.1088/0268-1242/27/4/045005
Photoresponse of indium oxide particulate-based thin films fabricated using milled nanorods grown by the self-catalytic vapor–liquid–solid process L Qin, P S Dutta and S Sawyer
Electrical, Computer, and Systems Engineering Department, Rensselaer Polytechnic Institute, Troy, NY 12180, USA
Received 28 November 2011, in final form 30 January 2012 Published 22 February 2012 Online at stacks.iop.org/SST/27/045005
Abstract Indium oxide (In2O3) nanorods were grown on silica substrates by using the self-catalytic vapor–liquid–solid growth process. The photoresponse of the nanorods was compared to that of the thin film, tin-doped indium oxide (ITO). The nanorods demonstrated a wavelength-dependent photoresponse with high responsivity of 1.82 A W−1 at 405 nm. In contrast, the conductive ITO thin film did not show a photoresponse to light. Analysis results showed that different surface states of materials as well as doping in ITO contributed to the significant difference in the photoresponse of samples.
(Some figures may appear in colour only in the online journal)
Indium oxide (In2O3) is an amphoteric oxide of indium with bixbyite-type cubic crystals. Its documented bandgap value has recently been revised from the old value 3.7 to 2.9 eV [1, 2]. As an intrinsic n-type semiconductor, In2O3 has been used as a resistive element in integrated circuits and heterojunction structure with indium phosphide (InP) and gallium arsenide (GaAs) . In combination with tin dioxide (SnO2), In2O3 forms tin-doped indium oxide (ITO), a material used for transparent conductive coatings. The performance of In2O3 as a conductive material is well studied. However, its semiconductor properties are not fully understood. Many previous studies mainly focused on the preparations and optical properties (especially light emission) of In2O3 nanomaterials due to their beneficial properties, such as quantum confinement effect, high surface area to volume ratio, better absorption than bulk material and high quantum efficiency [4–6]. Currently, electrodeposition by anodic alumina nanoporous structure templates, laser ablation and sol–gel techniques have been used in the synthesis of In2O3 nanostructures [1, 4–6]. Research on electrical and optical properties of In2O3 nanomaterials is growing [7–12];
however, the photoelectric performance of In2O3, to the best of our knowledge, has not been studied yet.
In this paper, In2O3 nanorods are synthesized by the self-catalytic vapor–liquid–solid (VLS) growth process. The photoresponse characteristics of In2O3 nanorods are measured and compared to those of In2O3 thin films with different conductivities. The following analysis shows that surface states in the nanorods cause a change in the Schottky barrier height resulting in a difference in the photoresponse performance.
2. Sample preparation
The In2O3 synthesis using a VLS technique was carried out at 1200 ◦C in continuously flowing oxygen ambient in a tubular furnace. The precursors used for the growth of nanorods were high purity (7N pure) indium films coated around a silica (quartz) tube. The entire growth process occurred within 3–4 h after the furnace reached the growth temperature of 1200 ◦C. At the end of the growth process, loosened yellow colored In2O3 nanorods were grown along the silica tube. The XRD pattern of as-grown nanorods was taken by a Bruker
0268-1242/12/045005+06$33.00 1 © 2012 IOP Publishing Ltd Printed in the UK & the USA
http://dx.doi.org/10.1088/0268-1242/27/4/045005 mailto:firstname.lastname@example.org http://stacks.iop.org/SST/27/045005
Semicond. Sci. Technol. 27 (2012) 045005 L Qin et al
Figure 1. XRD patterns of as-grown In2O3 nanorods.
Figure 2. SEM images of In2O3 nanorods before and after grinding (inset).
D8 Discover x-ray diffractometer, as shown in figure 1. The crystalline peaks match with the diffraction data of cubic indium oxide (AMCSD 0017267, a = b = c = 10.12 Å, α = β = γ = 90◦) of high purity. It confirms that the as-grown nanorods are indeed In2O3.
The structure and morphology of the In2O3 nanorods were then further analyzed by using a Carl Zeiss Ultra 1540 dual beam scanning electron microscope with an accelerating voltage of 5 kV. The images are shown in figure 2, from which we can see that the as-grown nanorods have a wide range distribution in size and length. To prepare shorter nanorods to better deposit onto any substrate for electrical and optical measurements, the synthesized nanorods were ground. After grinding (inset of figure 2), the nanorods were broken into smaller rods significantly, but more surface defects were introduced during the grinding. An attempt to eliminate some of those surface defects was made through annealing in air at 1200 ◦C for 2–6 h.
Table 1. Parameters of LEDs used in the experiment.
Peak wavelength Total optical power (nm) within active area (mW)
280 nm 0.3364 340 nm 0.2168 405 nm 0.0358 470 nm 0.0237
The nanorods were then divided into three batches. The first batch (sample A) was dispersed in DI water, coated onto the quartz substrate and then naturally dried in air. A thin film with uniformly distributed In2O3 well attached onto the quartz was formed. The second (sample B) and the third (sample C) batches were dispersed in a polyvinyl alcohol (PVA) solution (at 100 ◦C) with a weight ratio of In2O3 to PVA equal to 100:1 and 10:1, respectively. These mixtures were deposited onto quartz substrates and dried in air. Sample B produced a thin film with non-uniform distribution of In2O3 though the thin film attached well to the quartz substrate. Sample C produced a uniform plastic thin film with In2O3 uniformly distributed, but the film was completely separated from the quartz substrate. A picture of the three samples is shown in figure 3(a). The surface morphology and particle distribution of the three samples are shown in the SEM images in figure 3(b).
3. Results and discussion
UV–Vis absorption spectra were recorded using a Shimadzu UV–Vis 2550 spectrophotometer in the wavelength range of 200–800 nm. As demonstrated in figure 4, the cut-off wavelengths of In2O3 nanorods before and after grinding are the same, about 425 nm (2.9 eV), which is also the same wavelength as that of bulk material. The In2O3 nanorods after grinding exhibit an increase in the absorption intensity since smaller size materials are easily attached to and more uniformly distributed onto the quartz substrate.
As shown in the inset of figure 5(a), point contact current–voltage (I–V) characteristics and the time-resolved photocurrent of samples were measured using a HP4155B semiconductor parameter analyzer under dark and illumination conditions at room temperature in air. The light sources used were light-emitting diodes (LEDs) with parameters listed in table 1. The active areas of samples were 0.007 85 cm2. Figures 5(a)–(d) represent the typical I–V curves of samples A, B, C and ITO, respectively, with cut-off wavelength at 300 nm which is shown in the inset of figure 5(d). Figure 5(e) shows a rough spectral responsivity of sample A biased at −20 V based on the information given by figure 5(a).
The nonlinear I–V responses in figures 5(a)–(c) show signatures of rectifying effects between the In2O3 nanorods and the tungsten needles of the semiconductor parameter analyzer. This rectifying behavior decreases as the conductivity of sample increases (due to the presence of PVA connecting the nanorods, as shown in figures 1(b) and (c)). The contacts between ITO and tungsten are ohmic as expected. These results indicate that the current conduction mechanism in ITO is different from that in samples A, B and C.
Semicond. Sci. Technol. 27 (2012) 045005 L Qin et al
Figure 3. (a) Picture and (b) SEM images of samples A (In2O3), B (In2O3 : PVA = 100:1) and C (In2O3 : PVA = 10:1) (from left to right).
Figure 4. Absorption spectra of In2O3 nanorods demonstrate a cut-off wavelength at 425 nm (2.9 eV).
One important parameter to represent the rectified effect of Schottky contact is the barrier height φB. Based on the thermal emission assumption, the barrier height is given by
φB = −kT q
) , (1)
where Is is given by the average dark currents when the applied voltage is 0 . The active area A is 0.007 85 cm2. The Ri